**FFI RAPPORT**

**INVERSE MODELING OF PENETRATION** **INTO 12.7 CARTRIDGES**

NILSSEN Jan R, MOXNES John F

**FFI/RAPPORT-2002/02386**

**Documents** ^{PDF}

^{PDF}

**Complete**

**Click Here & Upgrade**
**Expanded Features**
**Unlimited Pages**

FFIBM/778/130

Approved

Kjeller 14 May 2002

Bjarne Haugstad Director of Research

**INVERSE MODELING OF PENETRATION INTO**
**12.7 CARTRIDGES**

NILSSEN Jan R, MOXNES John F

FFI/RAPPORT-2002/02386

**FORSVARETS FORSKNINGSINSTITUTT**
**Norwegian Defence Research Establishment**
P O Box 25, NO-2027 Kjeller, Norway

**Documents** ^{PDF}

^{PDF}

**Complete**

**Click Here & Upgrade**
**Expanded Features**
**Unlimited Pages**

**FORSVARETS FORSKNINGSINSTITUTT (FFI)** ** UNCLASSIFIED**

**Norwegian ****Defence ****Research ****Establishment ** **_______________________________**

**P O BOX 25** **SECURITY CLASSIFICATION OF THIS PAGE**

**N0-2027 KJELLER, NORWAY** **(when data entered)**

**REPORT DOCUMENTATION PAGE**

**1) PUBL/REPORT ****NUMBER** **2) ** **SECURITY ****CLASSIFICATION** **3) NUMBER OF**

FFI/RAPPORT-2002/02386 UNCLASSIFIED ^{ PAGES}

**1a) PROJECT ****REFERENCE** **2a) DECLASSIFICATION/DOWNGRADING ****SCHEDULE** 15

FFIBM/778/130 -

**4) TITLE**

INVERSE MODELLING OF PENETRATION INTO 12.7 CARTRIDGES

**5) ** **NAMES OF AUTHOR(S) IN FULL (surnam e first)**

NILSSEN Jan R, MOXNES John F

**6) ** **DISTRIBUTION ****STATEMENT**

Approved for public release. Distribution unlimited. (Offentlig tilgjengelig)

**7) ** **INDEXING ****TERMS**

**IN ****ENGLISH:** **IN ****NORWEGIAN:**

** a)** Brass ** a)** Messing

** b)** Penetration ** b)** Penetrasjon

** c)** Inverse modeling ** c)** Invers modellering

** d)** ** d)**

** e)** ** e)**

**THESAURUS REFERENCE:**

**8) ABSTRACT**

In this article a study of the forces caused by penetration of steel penetrators into cartridges of brass has been carried out. Experimental data was compared with simulations using the Nike-2D code and with solutions from a provided cavity expansion theory for thin cylindrical shells.

The Nike-2D simulations gave good agreement with the experimental results. By using an inverse modeling technique a constitutive model of the brass was established.

**9) DATE** **AUTHORIZED BY** **POSITION**

This page only

14 May 2002 Bjarne Haugstad Director of Research
**UNCLASSIFIED**

**SECURITY CLASSIFICATION OF THIS PAGE**
**(when data entered)**

**Documents** ^{PDF}

^{PDF}

**Complete**

**Click Here & Upgrade**
**Expanded Features**
**Unlimited Pages**

**CONTENTS**

**Page**

1 INTRODUCTION 7

2 THE EXPERIMENTAL SET-UP 7

3 THE ANALYTICAL PENETRATION THEORY 8

4 NIKE RESULTS, ANALYTICAL RESULTS AND EXPERIMENTAL

RESULTS 10

5 CONCLUSION/DISCUSSION 11

References 11

APPENDIX

A APPENDIX 12

B APPENDIX 13

Distribution list 15

**Documents** ^{PDF}

^{PDF}

**Complete**

**Click Here & Upgrade**
**Expanded Features**
**Unlimited Pages**

**INVERSE MODELING OF PENETRATION INTO 12.7 CARTRIDGES**

**1** **INTRODUCTION**

The Norwegian armed forces use the Multipurpose 12.7 ammunition. Nammo Raufoss AS is the inventor of the Multipurpose (MP) concept, and the MP technology was developed during the end of the 60s. The first series production started in the beginning of the 70s.

During 2001 a contact between FFI and the Norwegian Army was signed. One of the

objectives was to analyze in more detail some of the mal-functions of the gun, which has been observed during launch. Of special interest were events behind gunpowder gas leakage caused by rupturing of the cartridge during launch. In order to analyze this phenomenon by numerical calculations, the material model of the brass cartridge must be established.

In order to find the material model of the brass cartridge during large extension, a new non- standard test where a steel penetrator was forced into the empty cartridge has been analyzed.

Simulation results from the Nike 2D[1] code and from analytical calculations were compared with the experimental results of the force and displacement of the penetrator entering into the brass cartridge. A material model of the brass was achieved by searching for a material model that gave close agreement with the experiment and the numerical calculations, a so-called inverse modeling technique. The constructed material model is in good agreement with other models reported in the literature and with the hardness test.

**2** **THE EXPERIMENTAL SET-UP**
In figure 2.1 the experimental set-up is shown.

*Figure 2.1 * *The experimental set-up of the penetrator entering a cartridge*

The experimental recording was the force and the displacement of the penetrator.

8

**3** **THE ANALYTICAL PENETRATION THEORY**

This section gives a short description of the constructed penetration theory for penetration into thin cylindrical shells.

Assume that initially the inside diameter of cylindrical shell is equal to the diameter of the conical penetrator so that physical contact is established.

Let *F* be the force on the penetrator. The sum of mechanical and friction forces give the total
force, i.e.

*def*

*s* *f*

*F* =*F* +*F* . According to the standard cavity theory, which applies to a semi-
infinite medium the normal stress on the surface of the penetrator is

(2 / 3) (1 [2 / ])

*n* *t* *t*

*mod*

*Y* *Log* *G Y*

σ = + (3.1)

where

σ*n*: Normal stress
*G*: Shear modulus
*Y**t*: Yield limit in target

This normal stress is different for a cylindrical shell. Assume the parameters
*R* : Average radii of the cylindrical shell

*h*: Thickness of the shell

The stresses during the initial elastic phase is at the inside surface of the shell given by

(1/ 2) / ,

(1/ 6) / , (1/ 3) /

*rr*

*rr*

*mod* *mod*

*p R h* *p*

*s* *s* *p R h s* *p R h*

θθ ϑϑ

θθ θθ

σ =σ = σ = −

= ≈ ≈ −

(3.2)

where

*p*: Inside pressure of the shell

Assuming that after the initial elastic phase the shell yields essentially over the complete thickness, gives from (3.2) and assuming a Mises material, that

**Documents** ^{PDF}

^{PDF}

**Complete**

**Click Here & Upgrade**
**Expanded Features**
**Unlimited Pages**

2 2 2 2

(3 / 2)( * _{rr}* )

*4*

_{t}*/*

_{t}*mod*

*s* +*s*_{θθ} +*s*_{ϑϑ} = *Y* ⇒ =*p* *Y h R* (3.3)

The average radial stress over a thickness of the shell is given as ,σ ≈* _{rr}* (1/ 2)

*p*. Using this value as the normal stress gives the mechanical strength force as

( ) 2 ( / )

*s* *n* *n* *p* *t* *p*

*Ap*

*F* σ *Cos*θ *dA* σ *dA* *Y h R A*

Ω

=

### ∫

=### ∫

=_{(3.4)}

where

θ:= angle between the normal stress vector on the surface of the penetrator and the axial direction

Ω: contact surface between the penetrator and the steel plate
*dA*: surface element

*dA**p*: projected surface element

*A**p*: projected contact area between the penetrator and the plate in the direction of penetration
The friction force is given as

*f* *n* ( )

*F* σ µ*Sin*θ *dA*

Ω

=

### ∫

^{(3.5)}

where

µ: coefficient of friction

Assuming conical half angleψit follows that the friction force is given by

/ ( )

*f* *s*

*F* =µ*F Tan*ψ (3.6)

Let *A d** _{p}*( ) be the projected area of the penetrator into the target as a function of the

penetration depth after contact between the hollow cylindrical shell and the conical penetrator.

Equations (3.4) and (3.6) then give the total force as

2 2

1 1

( ) 2 ( / )(1 / ( )) * _{p}*( ),

*( ) ( ( ) )*

_{p}*F d* = *Y h R* +µ *Tan*ψ *A d A d* ≈π *R Tan*+ ψ *d* −π*R* (3.7)
where the projected area can be established from a simple drawing of the situation.

10

**4** **NIKE RESULTS, ANALYTICAL RESULTS AND EXPERIMENTAL RESULTS**
In this section simulations with Nike-2D will be compared with experiments and with results
from the presented penetration theory. Figure 4.1 shows the Lagrange grid of the target and of
the penetrator.

*Figure 4.1 * *The simulated Lagrangian grid*

Figure 4.2 shows three different curves. The simulated force, the experimental force, and the analytical force from equation (3.7), all as a function of the penetration depth.

*Figure 4.2 * *The force as a function of the displacement*

**Documents** ^{PDF}

^{PDF}

**Complete**

**Click Here & Upgrade**
**Expanded Features**
**Unlimited Pages**

We observe that the agreement between the curves is very good. The simulation result deviates from the experimental results in the final part of the penetration process. The effect is probably caused by numerical instability. The established material parameters are given in appendix A.

**5** **CONCLUSION/DISCUSSION**

We found in the last section that the Nike-2D and the analytical theory show good agreement with experiments. The provided inverse modelling technique also gave good agreement with the constructed analytical theory. The material properties of the brass are in agreements with values in the literature. The Brinell hardness in area 10 is close 150,which gives a yield strength of 340 MPa for Cu.

**References**

[1] Nike-2D user Manual.

**Acknowledgement: We thank Eva Friis at Nammo Raufoss for helping us with the input to**
the Nike 2d code, and Svein W Eriksen and Finn Risebrobakken at FFI for doing the hardness
tests.

12

**A** **APPENDIX**

The following material parameters were found for the brass

Brass density: 8.31 g/cm^3,Youngs modulus: 1.15 10^11 Pa, Poison ratio: 0.3 Yield function ( piece wise linear): Strain: 0.0, 0.1, 0.2, 0.3,0.5,0.8,1.1,5.0 Stress (GPa):0.335, 0.371,0.398,0.418,0.449,0.485,0.514,0.712

The material properties is in good agreement with other brass materials ( Jacket 12.7). A yield strength of 340 MPa corresponds with a hardness of 150 Brinell for Cu.

**Documents** ^{PDF}

^{PDF}

**Complete**

**Click Here & Upgrade**
**Expanded Features**
**Unlimited Pages**

**B** **APPENDIX**

Hardness and chemical analyses of 12.7 cartridges.

Hardness as a function of position from the cartridge edge is measured for 3 different used cartridges. The chemical analysis is performed by using the electron microscope.

Cartridge-1:FNB 00, Cartridge-2:FNB 00,Cartridge-3:FNB 91

Cartridge-3 has a crack. The measurements in series 2 go along this crack.

Dates 7-10 are near the crack (approximately 5 mm from the crack)

Cartridge-1 1 2 3 4 5 6 7 8 9 10 Series-1 110 139 126 149 165 171 170 156 151 141 Brinell Cartridge-2 1 2 3 4 5 6 7 8 9 10

Series-1 134 137 148 158 - - - - - - Brinell Series-2 100 117 139 148 147 - - - - 168 Brinell

Cartridge-3 1 2 3 4 5 6 7 8 9 10 Series-1 137 135 123 130 147 160 164 165 159 151 Brinell Series-2 146 132 136 140 144 159 170 - 166 153 Brinell - means no measurements

*Figure B.1 * *Cartridge with the marked areas*

14

*Figure B.2 * *Brinell hardness as a function of area*

Chemical analysis of cartidge-3

Series-1 (close to the crack): Cu 70.71 % - 69.41 %, Average: 7 Zn 29.29 % - 30.59 %, Average: 29.94 %

Series-2 Cu 70.53 % - 69.45 Average: 69.99 %

Zn 29.47 % - The density is given by the formulae

1/ρ* _{CuZn}*30=0.7 /ρ

*+0.3 /ρ*

_{Cu}*(B.1)*

_{Zn}where

30

ρ*CuZn* : Density of cartridge

3 3

8.94 10 /

*Cu* *kg m*

ρ = : Density of Cu

3 3

7.14 10 /

*Zn* *kg m*

ρ = : Density of Zn

(B.1) then gives that

3 3

30 8.3110 /

*CuZn* *kg m*

ρ =

c1s1.dat c2s1.dat c2s2.dat c3s1.dat c3s2.dat

Area

10 9 8 7 6 5 4 3 2 1 Br

170

160

150

140

130

120

110

100

**Documents** ^{PDF}

^{PDF}

**Complete**

**Click Here & Upgrade**
**Expanded Features**
**Unlimited Pages**

**DISTRIBUTION LIST**

** FFIBM Dato: 14 mai 2002**

RAPPORTTYPE (KRYSS AV) RAPPORT NR. REFERANSE RAPPORTENS DATO

X ^{RAPP} ^{NOTAT} ^{RR} 2002/02386 FFIBM/778/130 14 mai 2002

RAPPORTENS BESKYTTELSESGRAD ANTALL EKS

UTSTEDT

ANTALL SIDER

Unclassified 35 15

RAPPORTENS TITTEL FORFATTER(E)

INVERSE MODELING OF PENETRATION INTO 12.7 CARTRIDGES

NILSSEN Jan R, MOXNES John F

FORDELING GODKJENT AV FORSKNINGSSJEF FORDELING GODKJENT AV AVDELINGSSJEF:

Bjarne Haugstad Jan Ivar Botnan

**EKSTERN FORDELING ** **INTERN FORDELING**

ANTALL EKS NR TIL ANTALL EKS NR TIL

Nammo Raufoss AS 14 FFI-Bibl

3 Gard Ødegårdstuen 1 Adm direktør/stabssjef Postboks 25, 2831 Raufoss 1 FFIE

1 FFISYS 1 FFIBM 1 FFIN

1 Bjarne Haugstad, FFIBM 1 Svein W Eriksen, FFIBM 1 John F Moxnes, FFIBM 1 Gunnar Ove Nevstad, FFIBM 6 FFIBM

3 HFK-AMK, Alf Øversveen

FFI-K1 Retningslinjer for fordeling og forsendelse er gitt i Oraklet, Bind I, Bestemmelser om publikasjoner for Forsvarets forskningsinstitutt, pkt 2 og 5. Benytt ny side om nødvendig.